NANOMATERIALS Chemically reversible isomerization of NANOMATERIALS Chemically reversible...
Embed Size (px)
Transcript of NANOMATERIALS Chemically reversible isomerization of NANOMATERIALS Chemically reversible...
Chemically reversible isomerization of inorganic clusters Curtis B. Williamson1*, Douglas R. Nevers1*, Andrew Nelson2, Ido Hadar3, Uri Banin3†, Tobias Hanrath1†, Richard D. Robinson2†
Structural transformations in molecules and solids have generally been studied in isolation, whereas intermediate systems have eluded characterization. We show that a pair of cadmium sulfide (CdS) cluster isomers provides an advantageous experimental platform to study isomerization in well-defined, atomically precise systems. The clusters coherently interconvert over an ~1–electron volt energy barrier with a 140–milli–electron volt shift in their excitonic energy gaps. There is a diffusionless, displacive reconfiguration of the inorganic core (solid-solid transformation) with first order (isomerization-like) transformation kinetics. Driven by a distortion of the ligand-binding motifs, the presence of hydroxyl species changes the surface energy via physisorption, which determines “phase” stability in this system. This reaction possesses essential characteristics of both solid-solid transformations and molecular isomerizations and bridges these disparate length scales.
P hase transitions in solids and molecular isomerizations occupy different extremes for structural rearrangements of a set of atoms proceeding alongmechanistic path- ways. Phase transformations are initiated
by nucleation events (1) that are difficult to de- fine and then propagate discontinuously from lattice defects with activated regions smaller than the crystalline grains (incoherent transformation) (2). Small-molecule isomerization is a discrete process, in which the activation volume of the transition state is comparable to the size of the molecule (coherent transformation). Studies of isomerization and solid-solid transformations have thus far proceeded largely independently. Efforts to identify a system bridging these trans- formations have been made by examining the transformation of domains of reduced size, such as nanocrystals. Transformations of nanocrystals (100 to 10,000 atoms) do not mirror molecular isomerization, in that bulk-like phase transition behavior extends to the nanometer-length scale, even down to ~2 nm (2). Here we investigate the structural transformations in semiconductor clus- ter molecules at the boundary between molecular isomerizations and solid-solid phase transitions in nanocrystals (Fig. 1) by studying magic-size clusters (MSCs) (~10 to 100 atoms), as proto- typical systems. Studies of these clusters (diam- eter < 2 nm) with distinct chemical formulas revealed that the cluster structures were strongly influenced by the surface termination (2–5).
Previous work has observed that certain types, or families, of MSCs can be converted into other MSCs (5–8). Thus far, however, experiments claim- ing to have observed structural reorganization have been primarily conducted in the solution phase. Clusters in solution are free to interact with each other and with unbound surfactants, monomers, or by-products, and these interac- tions promote mass transport and etching pro- cesses. For example, reports on InP clusters show irreversible structural changes, aggregation, and etching in the presence of high concentrations of amines (5). Such cases indicate a loss in the products’ compositional integrity and thus that the transformation is not an isomerization. Struc- tural transformations have been proposed for the same InP clusters at lower amine concentrations (5) and in CdS clusters after changes in temper- ature (6). In the former case, the assignment to a structural transformation was made by indirect methods (9) based on changes in 31P nuclearmag- netic resonance shifts. This measurement per- mitted identification of only ~20% of the atoms
in the cluster, none of which were directly asso- ciated with the surface ligands, and the experi- ment did not rule out the possibility of etching. Substantial changes in the 31P spectrum were observed in different solvents, bringing into question the dynamical stability of InP clusters in solution and, by extension, their status as isolated molecules undergoing discrete trans- formations. For the CdS clusters (6), the kinetics of incomplete transformations between cluster types indicated a very high activation energy (~3 eV), which is likely too large to account for merely structural reorganization energies and points instead to interparticle interactions. A primary complication of these solution-phase studies has been the lack of direct characterization of atomic structure, such as x-ray total scattering, in the native environment of transformation (5, 6) that can be used to identify the existence and extent of a structural transformation (9). We demonstrate that a class of MSCs whose
local structures can be modeled with a composi- tion of Cd37S20 undergoes reversible isomeriza- tion between two discrete and stable states via a chemically induced, diffusionless transformation. We preserved the composition by isolating our clusters in solid films and determined the cluster structures (fit residuals < 0.2) through analysis of their x-ray pair distribution functions (PDFs). Switching between the isomers was triggered by the absorption-desorption of water or alcohol (hydroxyl groups) with an activation barrier of ~1 eV in both directions. This chemically in- duced, reversible transformation has charac- teristics of both molecular isomerization and bulk solid-solid transformations. These clusters are an attractive starting point for merging the long- and short-length scale descriptions of such transformations as mediated by the external surface energy. We synthesized high-purity clusters (i.e., single
product), characterized by a narrow excitonic absorption peak at 324 nm with negligible longer-wavelength absorption, via our high- concentration method (10). These clusters are stabilized by their mesophase (11) and immobi- lized in a thin solid film (Fig. 2A). We refer to this cluster type as a-Cd37S20. After exposure of
Williamson et al., Science 363, 731–735 (2019) 15 February 2019 1 of 5
1Robert F. Smith School of Chemical and Biomolecular Engineering, Cornell University, Ithaca, NY, USA. 2Department of Materials Science and Engineering, Cornell University, Ithaca, NY, USA. 3Institute of Chemistry and the Center for Nanoscience and Nanotechnology, The Hebrew University, Jerusalem 91904, Israel. *These authors contributed equally to this work. †Corresponding author. Email: email@example.com (U.B.); firstname.lastname@example.org (T.H.); email@example.com (R.D.R.)
Fig. 1. Inorganic isomerization. Isomerization is well established in small organic molecules (e.g., the cis-to-trans transformation of azobenzene), whereas bulk inorganic solids exhibit phase transformations. Although small in size, nanocrystals follow bulk-like behavior in their solid-solid transformations. At even smaller length scales, inorganic clusters isomerize with molecular- and inorganic solid–like characteristics. Red and blue indicate two different structures.
on A ugust 20, 2020
ow nloaded from
a-Cd37S20 films to methanol vapor, the exciton (first absorption) peak diminished, and a second narrow absorption peak emerged at 313 nm, in- dicating formation of the new species, b-Cd37S20, with an energy gap that is larger by 140 meV. Hereafter, only transformations with methanol are discussed in detail, but any hydroxyl-bearing species (alcohol or water) can initiate conversion of a to b. The b-Cd37S20 could be transformed back to
a-Cd37S20 (reversion) by purging the methanol and heating the MSC film (>60°C), and the re- version rate increased with temperature. We demonstrated a high degree of reversibility with four complete conversion-reversion cycles (inset of Fig. 2A) in the MSC isomerization without creation of other MSC families or nanocrystals (fig. S1D). This behavior in MSCs is reminiscent of reversible isomerization reactions, which are well known in small molecules (12). We observed that differences in the dielectric environment only weakly alter the absorption maximum wave-
length and that, indeed, the presence of hydroxyl- bearing species exclusively determines the favored isomer under the temperatures applied here. a-Cd37S20 may be stabilized at lower tem- peratures by maintaining an anhydrous envi- ronment, and b-Cd37S20 may be stabilized at higher temperatures (e.g., up to the boiling point of methanol) by maintaining the saturation of hydroxyl-bearing species. The stabilization of different MSC forms within a mesophase may have interesting consequences for nanopar- ticle formation once growth (e.g., by oriented attachment) is initiated, as mentioned in recent reports (13). BothMSC isomers had lowphotoluminescence
(PL) quantum yields (
by Cd and S, respectively. PDF analysis is an effective tool for atomic modeling that resolves fine features and subtle differences between data. Although powerful for low-symmetry and disordered systems, extracting atomic positions from PDF analysis and modeling hinges on the accuracy of the initial inputs (15, 16). Repeated fitting showed that a- and b-Cd37S20 structures occupied distinct energy minima whose separa- tion greatly exceeded possible overlap from thermal displacements, so that the clusters’ struc- tures are unambiguously different (fig. S2D). Simulations including contributions from the organic ligands and the mesophase assembly determined that the organic ligand shell does not substantially contribute to scattering above Q = 1.5 Å−1, where scattering from the inorganic structure is dominant, so that fittingG(r) beyond 2 Å even wit